Quartz Binding Peptides as Molecular Linkers towards
Fabricating Multifunctional Micropatterned Substrates
By Turgay Kacar, John Ray, Mustafa Gungormus, Ersin Emre Oren,
Candan Tamerler, and Mehmet Sarikaya*
Protein microarray technologies, used in proteomics and clinic used for the immobilization of nanoparticles and biomole-
assays, require efﬁcient patterning of biomolecules on selected cules.[13–15] Such peptides were either isolated from the hard
substrates.[1–3] Fabrication of these microarrays is possible tissues of the organisms, such as diatoms, or selected against a
provided that the proteins are spatially immobilized on an speciﬁc inorganic target using combinatorial molecular biology
inorganic surface via various lithography techniques, e.g., soft protocols, such as phage[13,15,16] or cell-surface displays.[17,18] In
lithography, dip-pen lithography, and photolithography. the literature, there are numerous peptide sequences already
Within the last decade, protein immobilization became a key selected for different inorganic substrates and used in proof-of-
issue in bio-nanotechnology, since immobilization provides principle applications, e.g. GaAs Pt, Au, Cu2O,
physical support to the molecule, resulting in improved stability ZnO, quartz (SiO2), Ag, TiO2, and zeolite. There
and activity and, furthermore, helps to separate proteins from has been a surge of research activity utilizing these genetically
solution, rendering them reusable.[7,8] The approaches for bio- engineered peptides for inorganics (GEPI), which could be
molecule immobilization on glass or metal substrates generally used for synthesis, binding, assembly, and linking of inorganic
require surface functionalization by self-assembled monolayers nanostructures, all under ambient conditions. These engineered
(SAMs) of bifunctional molecules, such as aminoalkylalkoxysi- peptides are also useful for functional electronics and optical
lanes for silica and carboxyl-terminated alkanethiols for gold devices.[13,15] Furthermore, the utility of genetically selected
substrates.[9,10] Despite their widespread utility, these traditionally peptides are desirable in immobilization not only for their high
available bifunctional molecules have certain limitations, such as inorganic-binding capability but also their high substrate and
causing random orientation of the protein on solid surface and biomolecular speciﬁcity. For example, using gold binding
requiring multistep chemical reactions, and the assembled peptides as linkers, functional proteins[12,23] and gold nanopar-
monolayers can be unstable during immobilization.[11,12] To ticles were immobilized on gold surfaces. Using these
overcome these limitations, it is preferable to have molecules as peptides, synthesis of SiO2, Ag, and Au nanoparticles,
direct linkers to the solid substrate of interest that not only have all and hybrid protein-Cu2O nanostructures have also been
the desired features of the conventional chemically prepared demonstrated.
SAMs but also have speciﬁcity to a given solid substrate and Polydimethylsiloxane (PDMS) stamping,[4,27] used for pattern-
assemble onto it efﬁciently. As we demonstrate in this work, ing of SAMs of alkanethiols on gold surfaces, is a common
biomolecules, in particular peptides, can provide the multi- soft-lithography technique for fabricating protein patterns.[28–33]
functionality of such a desired linker with high structural stability. PDMS stamping has been successfully used to prepare scaffolds
Molecular constructs based on peptides can be designed with for cell growth, nanotube formation, nanowire organiza-
bifunctionality, including a solid-substrate-binding ability and tion, microﬂuidic systems, and biosensing. In general,
incorporating a target molecule aligned consistently to carry out a silane- or thiol-based bifunctional molecules are used in these
desired function. studies for attachments of biomolecules on solid supports such as
Recently, an alternative technique emerged in which the glass or gold, respectively.[31,32,39–41] Using microcontact printing,
peptides with strong binding afﬁnity to inorganic surfaces were we and others have demonstrated printing of gold-binding
peptides on gold substrates for directed immobilization of gold
[*] Prof. M. Sarikaya, T. Kacar, J. Ray, M. Gungormus, Dr. E. E. Oren,
nanoparticles, streptavidin-functionalized quantum dots,
Prof. C. Tamerler and proteins, e.g., enhanced green ﬂuorescent protein.
Genetically Engineered Materials Science and Engineering Center In this study, we show micropatterning of two different
Department of Materials Science and Engineering photoactive target molecules, ﬂuorescent quantum-dot nanocrys-
University of Washington tals and ﬂuorescein, on quartz surface, immobilized via
Seattle WA 98195 (USA)
E-mail: firstname.lastname@example.org quartz-binding peptides (see Experimental). The fabrication
T. Kacar, Prof. C. Tamerler process incorporates a combination of microcontact printing
Department of Molecular Biology and Genetics and directed self-assembly processes successively. The patterned
MOBGAM, Molecular Biology, Biotechnology substrates were examined using ﬂuorescence microscopy to
and Genetics Research Center demonstrate the bifunctionality and the quality of the pattern
Istanbul Technical University
Maslak Istanbul (Turkey)
fabrication. Our results show that the attachment of quantum
dots or photoactive molecules on a substrate is material-speciﬁc.
DOI: 10.1002/adma.200801877 For example, when silica is the substrate, a quartz-binding
Adv. Mater. 2009, 21, 295–299 ß 2009 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim 295
peptide (QBP) is used as the linker. To demonstrate the through a ﬂuorescein isocyanate (FITC) ﬁlter using a ﬂuores-
material-speciﬁcity of the QBP1, we show that it does not bind cence microscope. The result of this control experiment indicates
to a gold substrate. that the target molecule by itself has no afﬁnity to quartz
Quartz-binding peptides have been designed previously using substrate. We then used ﬂuorescein-conjugated molecule,
a knowledge-based approach. Here, we speciﬁcally use QBP1 and QBP1-F, as the molecular ink to produce a pattern on the quartz
QBP2 sequences that were chosen as strong and weak binders to substrate, following the stamping procedure shown in Figure 1a.
quartz surfaces, respectively (see Experimental). The molecular The ﬂuorescence microscopy image in Figure 1c clearly reveals
binding characteristics of these two peptides have been high contrast, in which the green lines are indicative of the
quantitatively determined using various techniques, including micropatterned QBP1-F molecules. Besides ﬂuorescein, the
surface plasmon resonance spectroscopy (SPR). Based on the procedure was repeated using an Albumin–ﬂuorescein isothio-
SPR data, the apparent adsorption rate constants (kobservable) of cyanate conjugate, BSA-F, as another control molecule (Support-
QBP1 and QBP2 were calculated to be 0.43 sÀ1 and 0.068 sÀ1, ing Information Fig. S2). Comparison between the ﬂuorescence
respectively. The kobservable values represent the initial adsorption intensity measurements recorded from these three samples (Fig.
rates for each of the peptides on the silica surface (Supporting 1b and c, and Supporting Information Fig. S2) clearly shows that
Information Fig. S1). For use as molecular inks in the PDMS the QBP1-mediated ﬂuorescein-molecule immobilization was an
stamping experiments, both peptides were chemically synthe- order of magnitude more efﬁcient than that mediated by BSA
sized and were then either biotinylated, namely QBP-bio, or (Supporting Information Fig. S3). This result demonstrates the
conjugated with ﬂuorescein via the reactive isothiocyanate group, utility of the inorganic-binding peptide, i.e., QBP1, as a linker
QBP-F. The QBP-bio conjugates were then labeled with mediating the immobilization of a ﬂuorescent molecule,
ﬂuorescent quantum-dot nanocrystals (QD) linked to streptavidin ﬂuorescein, on silica using the microcontact-printing technique.
protein (SA-QD); here SA is known to have strong molecular Parallel to the ﬁrst experiment, we also used the biotinylated
recognition to biotin. QBP as an ink, again using microcontact printing to generate a
Our ﬁrst experiment demonstrates micropatterning of a micropattern of a probe, e.g., biotin, conjugated peptide. This
functional target molecule (ﬂuorescein) conjugated to QBP1 way, the fabricated pattern would be biofunctional against
onto a quartz surface using microcontact printing (Fig. 1). Figure streptavidin, and could be used as a template for the assembly
1a shows a schematic illustration describing the PDMS stamping of streptavidin-coated QDs through biotin-streptavidin molecular
of the QBP1-F conjugate molecules used as ink. In this recognition. In this case, we ﬁrst used a PBS buffer (phosphate
experiment, we chose ﬂuorescein as the target molecule, due buffered saline) alone as the control experiment, stamping it on
to its chromogenic property resulting in the emission of green the quartz surface using PDMS, to produce a PBS pattern that
light at l ¼ 530 nm. As a control, we ﬁrst attempted to stamp was then incubated by SA-QD. We ﬁnd that the PBS buffer alone
ﬂuorescein on the quartz substrate alone. As shown in Figure 1b, used as an ink does not allow immobilization of QDs (Supporting
we see no contrast when the patterned substrate was imaged Information Fig. S4). The utility of QBP-bio as a PDMS ink to
generate a functional micropattern is shown schematically in
Figure 2a. The micropatterned surface would then be incubated
with SA-functionalized QDs, allowing its directed immobilization
only on the stamped regions. We used both strong and weak
quartz binding peptides, i.e., QBP1-bio and QBP2-bio, respec-
tively, the latter being the negative control experiment. Figure 2b
and c demonstrate the afﬁnities of the quartz-binding peptides on
quartz surface. We carried out the experimental procedure
schematically described in Figure 2a using QBP1-bio as the
molecular linker for the successful directed immobilization of
SA-QD, as shown in Figure 2b. When QBP2-bio was used,
instead, as the ink in PDMS patterning, because of its weak
binding characteristics, no SA-QD immobilization was possible,
as demonstrated in the negative control experiment displayed in
Figure 2c. Finally, to demonstrate the material-speciﬁcity of
QBP1-bio for quartz, we used gold as the substrate, and repeated
the procedure. Again, as shown in Figure 2d and e, no SA-QD was
immobilized on the patterned gold substrate, using either the
strong- or the weak-binding peptide. These experiments indicate
that QBP1 has a unique material-speciﬁc property, at least
between quartz and gold substrates, in which it can immobilize
probe molecules (e.g., biotin) on quartz, rendering the surface
In the last demonstration of solid-binding peptide as a
Figure 1. a) Schematic representation for PDMS patterning of QBP1-F on molecular assembler, we use two different nano-entities, QDs and
quartz. Fluorescence microscopy images of the substrates after micro- ﬂuorescent molecules, and sequentially assemble them on a
patterning with b) ﬂuorescein alone, as the control, and with c) QBP1-F. micropatterned surface utilizing the material-speciﬁcity of the
296 ß 2009 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim Adv. Mater. 2009, 21, 295–299
inorganic-binding peptide. In this case, direc-
ted immobilization of the QDs is followed by
the GEPI-mediated assembly of the ﬂuorescent
molecule, using the procedure schematically
illustrated in Figure 3a. The directed immo-
bilization of SA-QD on a QBP1-bio-patterned
surface is shown in Figure 3b as red stripes,
imaged with a ﬂuorescent microscope using a
QD605 ﬁlter, revealing contrast similar to that
in Figure 2b. Here, the dark stripes represent
the regions originally unoccupied, exposing
the bare quartz surface (Fig. 2b or Fig. 3a(i)).
Next, following the procedure in Figure 3a, the
assembly of the ﬂuorescent molecule, i.e.,
ﬂuorescein, is mediated using the QBP1-F
molecular conjugate. The assembled conjugate
molecules are imaged, as shown in Figure 3c,
using a FITC ﬁlter. At this step, the QBP1-F
molecular conjugate diffuses towards the
regions of the substrate previously unoccu-
Figure 2. a) Schematic representation of PDMS patterning of QBP1-bio on a solid substrate. pied, after the initial directed immobilization
b) Fluorescence microscopy image of the micropattern formed through directed assembly of of QDs. Both images in Figure 3b and c were
SA-QD upon the PDMS stamped QBP1-bio on quartz. c) The experiment was repeated, as a recorded from the same area of the sample,
negative control, using the weak binder QBP2-bio as the ink, revealing no micropattern on the showing regular alternating lines of red and
surface. In d,e), the procedures in b) and c) were repeated on gold surfaces, respectively
green stripes, corresponding to the directed-
(substrate as the negative control). The results demonstrate the speciﬁcity of the strong
quartz-binding peptide as a true molecular linker, here used as a PDMS ink, on the quartz surface. assembled QDs and mediated-assembled
ﬂuorescein molecules, respectively. This result
demonstrates that the QBP1 sequence acts as
an efﬁcient molecular linker as well as a
versatile PDMS ink. Furthermore, we demon-
strate here the coassembly of two diverse nano-entities without
the involvement of complex surface modiﬁcation, often involved
in silane-based procedures.[11,40]
In conclusion, we present an application of inorganic
solid-binding peptides, used as ink for microcontact printing
as well as linker for self-assembly. We demonstrate that the
molecular constructs based on QBPs, e.g., QBP1, can be designed
with bifunctionality, including both a solid-substrate-binding
ability and incorporating a target molecule carrying out a robust
function. Here, we use either ﬂuorescein or biotin in QBP1-based
molecular constructs with nanophotonic or biomolecular
recognition functions. Furthermore, we demonstrate a procedure
involving microcontact printing and self-assembly, both enabled
using the inorganic-binding peptide. Using a combined
procedure, one can coassemble diverse multifunctional mole-
cular and nano-entities on micropatterned substrates, both at
ambient conditions. The process described here has a potential
utility in the efﬁcient preparation of microarrays without the
potential problems or limitations associated with the conven-
tional silane-based chemical methods.
Figure 3. a) Schematics of QBP1-F assembly on a quartz substrate pre-
patterned using QBP1-bio/SA-QD. b) Fluorescence microscopy image of a
micropattern of directed immobilized SA-QD via the QBP1-bio patterned
surface (similar to Fig. 2b). The image was recorded using a QD605 ﬁlter. Experimental
c) Fluorescence microscopy image of the micropattern formed by the
immobilization of QBP1-F conjugate on the unﬁlled microlines, using the Materials: SA-QD conjugates with an emission at 605 nm were
same substrate as in b). The image was recorded using a FITC ﬁlter. purchased from Invitrogen, Co., USA. Quartz (111) crystal wafers were
d) Digital overlay of the images b) and c), demonstrating the utility of QBP1 received from MTI, Co., USA.
both as a molecular ink for stamping, for directing the immobilization of In silico Peptide Design: In our previous study, we designed novel
QDs, and a mediated molecular assembler for a ﬂuorescent molecule. quartz-binding peptide sequences in silico, using a knowledge-based
Adv. Mater. 2009, 21, 295–299 ß 2009 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim 297
design protocol, developed by us . In summary, in this knowledge- Fluorescence Microscopy: The quartz substrates on glass slides were
based design approach, we utilized the binding characteristics of a set of mounted on a Nikon Eclipse TE-2000U Florescence Microscope (Nikon,
biocombinatorially selected peptides, and generated a set of new peptide Japan) coupled with a Hamamatsu ORCA-ER cooled charge-coupled device
sequences with enhanced binding functionalities. This new approach (CCD) camera. FITC (exciter 460–500, dichroic 505, emitter 510–560,
performs all-against-all comparisons of experimentally selected and charac- Nikon) and QD605 (exciter 320-460, dichroic 475, emitter 605/40nm
terized peptide sequences and scores the alignments using sequence Chroma Technology Co, Rockingham, USA) ﬁlter sets are used for QBP1-F
similarity scoring matrices. Next, we derived a novel scoring matrix, and SA-QD detection, respectively. The images are recorded through
QUARTZ I , which optimizes the similarities within the strong quartz- Metamorph Software (Universal Imaging, USA).
binding peptide sequences and the differences between the strong and
weak quartz-binding peptide sequences. Using QUARTZ I scoring matrix,
computer-generated random peptide sequences were compared to the
strong quartz-binding peptide sequences; the ones with the highest and Acknowledgements
lowest similarity scores have been chosen as the strong (QBP1:
This research was funded by NSF through an MRSEC at the University of
PPPWLPYMPPWS) and weak (QBP2: CINQEGAGSKDK) quartz-binding
Washington and partially by BioMaterial program. Partial support (TK and
peptides, respectively. Here, the similarity scores indicate that peptides
CT) was also provided by TR-SPO. We thank M. T. Zin, C. Maremma and
with signiﬁcant sequence similarity to strong quartz binders have strong
U. O. S. Seker (UW) for technical help. Supporting Information is available
afﬁnity to quartz surface (e.g., QBP1), whereas the peptides with no
online from Wiley InterScience or from the authors.
sequence similarity to strong quartz binders have no afﬁnity to quartz
surface (e.g., QBP2). The experimental validation of the binding afﬁnities of Received: July 4, 2008
the designed peptides displayed excellent agreement with the predictions. Revised: August 14, 2008
Moreover, we also observed that the designed sequence has the highest
afﬁnity compared to the strongest phage display selected peptide .
Peptide Synthesis: Peptides, QBP1 and QBP2, are prepared on Wang
resin via automated Fmoc peptide synthesis employing a CSBio 336s
peptide synthesizer and HBTU activation. The biotinylated peptides are
prepared using pre-activated biotin (Biotin-OPN, EMD Biosciences). Biotin  A. S. Blawas, W. M. Reichert, Biomaterials 1998, 19, 595.
is dissolved in 1:1 DMF:DMSO and incubated with the resin-bound peptide  M. Cretich, F. Damin, G. Pirri, M. Chiari, Biomol. Eng. 2006, 23, 77.
overnight. Addition of biotin was conﬁrmed by Ninhydrin test. The resulting  D. H. Min, M. Mrksich, Curr. Opin. Chem. Biol. 2004, 8, 554.
dry resin-bound peptides are cleaved, side-chain-deprotected using  Y. N. Xia, G. M. Whitesides, Annu. Rev. Mater. Sci. 1998, 28, 153.
Reagent K (TFA/thioanisole/H2O/phenol/ethanedithiol 82.5:5.0:5.0:5.0:2.5),  K. B. Lee, S. J. Park, C. A. Mirkin, J. C. Smith, M. Mrksich, Science 2002, 295,
and precipitated by cold ether. The obtained crude peptide is puriﬁed by 1702.
Reverse-phase high-performance liquid chromatography (HPLC, Gemini
 A. Revzin, R. J. Russell, V. K. Yadavalli, W. G. Koh, C. Deister, D. D. Hile, M.
10u C18 110A column). The puriﬁed peptide was checked by mass
B. Mellott, M. V. Pishko, Langmuir 2001, 17, 5440.
spectroscopy (MS) using matrix-assisted laser desorption/ionization–time
 D. G. Castner, B. D. Ratner, Surf. Sci. 2002, 500, 28.
of ﬂight (MALDI-TOF). See Supporting Information for HPLC and MS data
for pure QBP1-bio. QBP1-F was commercially synthesized (United  U. T. Bornscheuer, Angew. Chem. Int. Ed. 2003, 42, 3336.
Biochemical Research, USA).  M. Mrksich, G. M. Whitesides, Annu. Rev. Biophys. Biomol. Struct. 1996, 25, 55.
PDMS Stamping of Peptides: The PDMS stamps, kindly received from  E. Ostuni, L. Yan, G. M. Whitesides, Colloids Surf. B 1999, 15, 3.
M. T. Zin (UW), were fabricated by molding a mixture of polydimethyl  K. Fujiwara, H. Watarai, H. Itoh, E. Nakahama, N. Ogawa, Anal. Bioanal.
siloxane and curing agent (10:1, Sylgard 184, Dow Corning, USA) on the Chem. 2006, 386, 639.
surface of a patterned silanized master for 2 days at ambient conditions.  T. J. Park, S. Y. Lee, S. J. Lee, J. P. Park, K. S. Yang, K. B. Lee, S. Ko, J. B. Park,
The stamps are then washed several times with ethanol, heptane, and last T. Kim, S. K. Kim, Y. B. Shin, B. H. Chung, S. J. Ku, D. H. Kim, I. S. Choi,
with ethanol, and dried with inert gas before being used. Anal. Chem. 2006, 78, 7197.
The patterned side of the PDMS stamp is incubated with a peptide  M. Sarikaya, C. Tamerler, A. K. Y. Jen, K. Schulten, F. Baneyx, Nat. Mater.
conjugate or ﬂuorescein (54 mM) in PBS buffer for 5 min. The peptide 2003, 2, 577.
solution is removed by pipette from the surface of the stamp, which is then  L. L. Brott, R. R. Naik, D. J. Pikas, S. M. Kirkpatrick, D. W. Tomlin, P. W.
dried with inert gas following brief washing with DI water. Quartz and gold Whitlock, S. J. Clarson, M. O. Stone, Nature 2001, 413, 291.
substrates are cleaned using isopropanol and ethanol, and dried with inert  S. R. Whaley, D. S. English, E. L. Hu, P. F. Barbara, A. M. Belcher, Nature
gas. The clean substrate is then applied to the surface of the stamp and 2000, 405, 665.
pressed using force for 10 s. and left on the stamp surface for 1 min. The  U. O. S. Seker, B. Wilson, S. Dincer, I. W. Kim, E. E. Oren, J. S. Evans, C.
substrate is removed from the stamp and the patterned side is washed with Tamerler, M. Sarikaya, Langmuir 2007, 23, 7895.
DI water for 2 min and dried with inert gas.  S. Brown, Nat. Biotechnol. 1997, 15, 269.
Following the stamping of biotinylated peptides, SA-QDs (20 nM) in PBS  C. K. Thai, H. X. Dai, M. S. R. Sastry, M. Sarikaya, D. T. Schwartz, F. Baneyx,
buffer is drop-coated onto the substrate and incubated for 15 min. The
Biotechnol. Bioeng. 2004, 87, 129.
substrates were then rinsed with DI water for 2 min and dried with inert gas.
 E. E. Oren, C. Tamerler, D. Sahin, M. Hnilova, U. O. S. Seker, M. Sarikaya,
In order to produce micropatterns of two different target molecules, i.e.,
R. Samudrala, Bioinformatics 2007, 23, 2816.
QDs and ﬂuorescein, following SA-QD labeling, the quartz substrate was
 R. R. Naik, S. J. Stringer, G. Agarwal, S. E. Jones, M. O. Stone, Nat. Mater.
drop-coated with QBP1-F (54 mM) in PBS buffer and incubated for 15 min.
The substrate was again rinsed with DI water for 2 min and then dried with 2002, 1, 169.
inert gas.  K. I. Sano, H. Sasaki, K. Shiba, Langmuir 2005, 21, 3090.
Cleaning and Reuse of PDMS Stamps: Detergent and sonication are  S. Nygaard, R. Wendelbo, S. Brown, Adv. Mater. 2002, 14, 1853.
effective methods for removal of peptide molecules bound to the PDMS  R. G. Woodbury, C. Wendin, J. Clendenning, J. Melendez, J. Elkind, D.
stamp, making the stamp reusable. After the PDMS experiments, the Bartholomew, S. Brown, C. E. Furlong, Biosens. Bioelectron. 1998, 13, 1117.
stamp was washed with DI water and placed in a small Petri dish containing  M. T. Zin, H. Ma, M. Sarikaya, A. K. Y. Jen, Small 2005, 1, 698.
detergent prepared with 0.2% Triton X-100 in PBS buffer. Stamps were then  S. Brown, M. Sarikaya, E. Johnson, J. Mol. Biol. 2000, 299, 725.
sonicated for 10 min in order to remove unwanted particles from the  H. X. Dai, W. S. Choe, C. K. Thai, M. Sarikaya, B. A. Traxler, F. Baneyx, D. T.
surface. After sonication, stamps were again washed with ethanol and dried Schwartz, J. Am. Chem. Soc. 2005, 127, 15637.
with inert gas.  A. Kumar, G. M. Whitesides, Appl. Phys. Lett. 1993, 63, 2002.
298 ß 2009 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim Adv. Mater. 2009, 21, 295–299
 M. Pla-Roca, J. G. Fernandez, C. A. Mills, E. Martinez, J. Samitier, Langmuir  Y. K. Kim, S. J. Park, J. P. Koo, D. J. Oh, G. T. Kim, S. Hong, J. S. Ha,
2007, 23, 8614. Nanotechnology 2006, 17, 1375.
 A. Bernard, J. P. Renault, B. Michel, H. R. Bosshard, E. Delamarche, Adv.  J. C. McDonald, D. C. Duffy, J. R. Anderson, D. T. Chiu, H. K. Wu, O. J. A.
Mater. 2000, 12, 1067. Schueller, G. M. Whitesides, Electrophoresis 2000, 21, 27.
 J. L. Tan, J. Tien, C. S. Chen, Langmuir 2002, 18, 519.  J. Carlsson, F. Winquist, B. Danielsson, I. Lundstrom, Anal. Chim. Acta
 R. S. Kane, S. Takayama, E. Ostuni, D. E. Ingber, G. M. Whitesides, 2005, 547, 229.
Biomaterials 1999, 20, 2363.  E. Delamarche, C. Donzel, F. S. Kamounah, H. Wolf, M. Geissler, R. Stutz,
 Z. P. Yang, A. Chilkoti, Adv. Mater. 2000, 12, 413. P. Schmidt-Winkel, B. Michel, H. J. Mathieu, K. Schaumburg, Langmuir
 W. Inglis, G. H. W. Sanders, P. M. Williams, M. C. Davies, C. J. Roberts, S. J. 2003, 19, 8749.
B. Tendler, Langmuir 2001, 17, 7402.  J. Feng, C. Y. Gao, B. Wang, J. C. Shen, Thin Solid Films 2004, 460,
 M. Scholl, C. Sprossler, M. Denyer, M. Krause, K. Nakajima, A. Maelicke, W. 286.
Knoll, A. Offenhausser, J. Neurosci. Methods 2000, 104, 65.  K. E. Sapsford, F. S. Ligler, Biosens. Bioelectron. 2004, 19, 1045.
 L. Ding, W. W. Zhou, H. B. Chu, Z. Jin, Y. Zhang, Y. Li, Chem. Mater. 2006,  M. T. Zin, A. M. Munro, M. Gungormus, N. Y. Wong, H. Ma, C. Tamerler,
18, 4109. D. S. Ginger, M. Sarikaya, A. K. Y. Jen, J. Mater. Chem. 2007, 17, 866.
Adv. Mater. 2009, 21, 295–299 ß 2009 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim 299